1.
MODELING AND SIMULATION OF HIGH PRESSURE COMPOSITE CYLINDERS FOR HYDROGEN STORAGE by JIANBING HU A DISSERTATION Presented to the Faculty of the Graduate School of the MISSOURI UNIVERSITY OF SCIENCE AND TECHNOLOGY In Partial Fulfillment of the Requirements for the Degree DOCTOR OF PHILOSOPHY IN MECHANICAL ENGINEERING 2009 Approved by K. Chandrashekhara, Advisor Lokeswarappa R. Dharani Hai-Lung Tsai Gregory E. Hilmas William E. Showalter
3.
iii PUBLICATION DISSERTATION OPTION This dissertation has been prepared in the form of three papers for publication asfollows:Pages 7-47 have been published in ADVANCED COMPOSITE MATERIALS.Pages 48-87 have been published in INTERNATIONAL JOURNAL OF HYDROGEN ENERGY.Pages 88-128 intended to submit to INTERNATIONAL JOURNAL OF HYDROGEN ENERGY.
4.
iv ABSTRACT Composite hydrogen cylinders provide an efficient means of storage of hydrogen gasfor modern hydrogen vehicles. Safety issues arising from the high gas pressure,temperature variation, fire attack, and fracture failures are the main concerns. The focusof this study is to develop a Finite Element (FE) model to predict the performance ofcomposite cylinders subjected to extreme mechanical/thermal loadings and provideguidance for design optimization. In the first part of this work, a predictive FE model ofcomposite cylinders has been developed considering various mechanical and thermalloadings. Doubly-curved laminated shell theory, accounting for transverse sheardeformation and geometric nonlinearity, is used to model the composite cylinder wall. Aback-propagation Neural Network (NNk) model, which is capable of predicting thefailure pressure for arbitrarily specified loading conditions, has been developed. Also, thefailure types and effects of thermal loading are investigated. In the second part, acomprehensive FE model has been developed to predict the behavior of the cylindersubjected to flame impingements. A failure model based on Hashin’s theory has beenimplemented to detect various failure modes of the composite. Damage due to resin burn-out and mechanical degradation are also considered in the model. Numerical results arepresented for thermal damage, residual properties and resin content profile of thecylinder. In the third part, fracture behavior of the cylinder with an axial surface crack inthe liner has been studied using fracture mechanics and a global-local FE technique withconsideration of autofrettage effect. Results on the fracture parameters (K and J-integral)with various autofrettage levels, crack sizes and crack shapes are presented.
5.
v ACKNOWLEDGMENTS The author wishes to extend his deepest gratitude to his academic advisor, Dr. K.Chandrashekhara, for his continued guidance, advice, encouragement and financialsupport throughout the course of the investigation and successful completion of thisdissertation research. The author also wishes to extend his greatest appreciation to the members of theadvisory committee, Dr. Lokeswarappa. R. Dharani, Dr. Hai-Lung Tsai, Dr. Gregory E.Hilmas, and Dr. William E. Showalter for their advice and encouragement, and their timeand effort for review of this dissertation. Many thanks go to Dr. S. Sundararaman for his prior input in this research. Theauthor also appreciates the assistance from his fellow colleagues and friends, Mr. JianChen, Mr. V.G.K. Menta and Mr. R. Vuppalapati. The author would like to take this opportunity to thank Mr. William Chernicoff of theUS Department of Transportation for his assistance with information and ideas. Thefunding of this research by the US Department of Transportation is gratefullyacknowledged. The author would also like to acknowledge the financial support received from theDepartment of Mechanical and Aerospace Engineering at Missouri S&T for GraduateResearch Assistantship and Graduate Teaching Assistantship. Finally, the author wishes to express his deepest gratitude to his parents, his sistersand brothers-in-law for their understanding, patience, encouragement, support, and forhelping realize and accomplish his dreams.
6.
vi TABLE OF CONTENTS PagePUBLICATION DISSERTATION OPTION ................................................................ iiiABSTRACT ..................................................................................................................ivACKNOWLEDGMENTS ..............................................................................................vLIST OF ILLUSTRATIONS .........................................................................................ixLIST OF TABLES ........................................................................................................xiSECTION1. INTRODUCTION ......................................................................................................11.1. BACKGROUND .....................................................................................................11.2. SCOPE AND OBJECTIVES ...................................................................................31.3. CONCLUDING REMARKS ..................................................................................5PAPER I. FAILURE PRESSURE PREDICTION OF COMPOSITE CYLINDERS FOR HYDROGEN STORAGE USING THERMO-MECHANICAL ANALYSIS AND NEURAL NETWORK ...........................................................................................7 ABSTRACT ..........................................................................................................7 1. INTRODUCTION .............................................................................................8 2. SHEAR DEFORMABLE SHELL THEORY ...................................................10 3. COMPOSITE FAILURE MODEL ...................................................................13 4. MATERIAL PROPERTIES .............................................................................14 5. FINITE ELEMENT SIMULATION .................................................................15 6. NEURAL NETWORK MODEL ......................................................................17 7. RESULTS AND DISCUSSION .......................................................................19 8. CONCLUSIONS .............................................................................................22 REFERENCES ....................................................................................................23 II. ANALYSIS OF COMPOSITE HYDROGEN STORAGE CYLINDERS SUBJECTED TO LOCALIZED FLAME IMPINGEMENTS ..............................48 ABSTRACT .......................................................................................................48 1. INTRODUCTION ..........................................................................................49 2. MODELING OF HIGH PRESSURE COMPOSITE HYDROGEN STORAGE CYLINDERS ..................................................................................................51
7.
vii 2.1. Thermal Model .........................................................................................51 2.2. Sub-laminate Model .................................................................................53 2.3. Formulation of Finite Element Model .......................................................55 3. MATERIAL MODELS ....................................................................................56 3.1. Temperature Dependent Material Properties .............................................56 3.2. Composite Failure Criteria ........................................................................57 3.3. Model for Hydrogen Gas ..........................................................................58 4. FINITE ELEMENT SIMULATION PROCEDURE .........................................59 5. RESULTS AND DISCUSSION .......................................................................60 6. CONCLUSIONS .............................................................................................62 REFERENCES ....................................................................................................63III. FRACTURE ANALYSIS OF HYDROGEN STORAGE COMPOSITE CYLINDERS WITH LINER CRACK ACCOUNTING FOR AUTOFRETTAGE EFFECT .............................................................................................................88 ABSTRACT .......................................................................................................88 1. INTRODUCTION ...........................................................................................89 2. METHODOLOGY ..........................................................................................91 2.1. Autofrettage Effect on High Pressure Composite Cylinder for Hydrogen Storage .....................................................................................................91 2.2. Stress Intensity Factor (K) Evaluation .......................................................93 2.3. J-Integral Evaluation ................................................................................94 2.4. Material Models ........................................................................................95 3. FINITE ELEMENT SIMULATION ...............................................................97 3.1. Global Model ............................................................................................98 3.2. Local Model .............................................................................................99 3.3. Simulation Procedure ..............................................................................100 4. RESULTS AND DISCUSSION .....................................................................101 4.1. Autofrettage Process Simulation ............................................................101 4.2. Stress Intensity Factor (K) and J-integral ...............................................102 4.3. Stress Field Characterization on the Crack Tip Vicinity .........................103 5. CONCLUSIONS ..........................................................................................104 REFERENCES .................................................................................................105
9.
ix LIST OF ILLUSTRATIONSFigure PagePAPER I1. Structure scheme of hydrogen storage cylinder .........................................................342. Doubly curved shell and coordinate system ...............................................................353. Finite element model of hydrogen cylinder ...............................................................364. Feedforward back-propagation Neural Network architecture .....................................375(a). Uniform thermal loading with Tin=Tout (in Case 1) ................................................385(b). Uniform thermal loading Tin=Tout (in Case 2) .......................................................395(c). Uniform thermal loading Tin=Tout (in Case 3) .......................................................406(a). Gradient thermal loading with Tout=50oC (in Case 1) ............................................416(b). Gradient thermal loading with Tout=50oC (in Case 2) ............................................426(c). Gradient thermal loading with Tout=50oC (in Case 3) ............................................437. Failure pressure with inside temperature variation (Tout=25oC) ..................................448. Ply-by-ply failure predictions under various thermal loadings ...................................459(a). Comparison of failure pressures from NNk and ABAQUS at = 15o ...................469(b). Comparison of failure pressures from NNk and ABAQUS at = 25o ...................47PAPER II1. Schematic of hydrogen cylinder ................................................................................732. Curve fitting for hydrogen gas state equation at constant density ...............................743. Finite element model of the cylinder .........................................................................754. Stacking sequence of the cylinder wall ......................................................................765. Finite element implementation schemes ....................................................................776. Variation of sink temperature with film coefficient ...................................................787. Internal pressure variation with time for various flame area sizes ..............................798. Temperature distributions along the length at inner surface of the aluminum liner .....809. Temperature distributions through composite thickness ............................................8110. Residual resin content through the thickness ...........................................................8211. Stress (S11) distribution through the thickness .........................................................8312. Stress (S22, S33) distribution through the thickness ...................................................8413(a). Fiber fracture index (Imt) contour around heat source ..........................................85
10.
x13(b). Matrix cracking index (Ift) contour around heat source .......................................8613(c). Density index (ρ/ρ0) contour around heat source .................................................87PAPER III1. Schematic of hydrogen composite cylinder .............................................................1122. Diagram of autofrettage process ..............................................................................1133. Schematic of domain integral evaluation .................................................................1144. Global finite element model ....................................................................................1155. Local finite element model ......................................................................................1166. Implementation scheme ..........................................................................................1177. von-Mises stress distribution in liner .......................................................................1188. Cyclic stress-strain curves for various autofrettage levels ........................................1199. Stress intensity factor (K) along crack front for various autofrettage levels .............12010. J-integral along crack front for various autofrettage levels ....................................12111. Stress intensity factor (K) against pressure loading for various autofrettage levels 12212. J-integral against pressure loading for various autofrettage levels ..........................12313. Stress intensity factor (K) along crack front with various geometric ratios ............12414. J-integral along crack front with various geometric ratios ......................................12515. Stress distribution of the crack front vicinity .........................................................12616. Transition of plastic zone shapes along crack front ................................................12717. Plastic zone shapes for various autofrettage levels .................................................128
11.
xi LIST OF TABLESTable PagePAPER I1. Ultimate strength of carbon/epoxy composite ...........................................................272. Mechanical and thermal properties of S-glass/epoxy .................................................283. Mechanical and thermal properties of Aluminum Alloy 6061-T6 ..............................294. Lay-up configurations for various winding patterns ..................................................305. Weights and biases for trained neural network ..........................................................316. Scale constants for trained neural network ................................................................327. Testing cases and maximum error of prediction ........................................................33PAPER II1. Curve fitting parameters for transverse and shear modulus ........................................672. Thermal expansion coefficients of carbon/epoxy .......................................................683. Specific heat and thermal conductivity of carbon/epoxy ............................................694. Parameters for resin reaction model ..........................................................................705. Strength of carbon/epoxy ..........................................................................................716. Design parameters for the cylinder ............................................................................72PAPER III1. Mechanical properties of carbon/epoxy composite ..................................................1102. Mechanical properties of Aluminum Alloy 7075-T651 ...........................................111
12.
1. INTRODUCTION1.1. BACKGROUND Currently, the energy crisis and environmental pollution arising from burning fossilfuel in vehicles are identified as some of the major concerns in the global world.Hydrogen, a renewable and clean energy resource, is a promising substitute for fossilfuels. One of the key challenges for the usage of hydrogen gas in automobiles is todevelop a compact and efficient way of hydrogen storage. The solutions for thischallenge can be categorized into three main groups [1-2]: (a) Cryogenic hydrogenstorage: It provides high volumetric density (0.07 kg/L) and good weight density (2.8 %),but liquefaction (-423.2 oF) is an intensive energy consuming process and evaporationreduces the gas usage efficiency. (b) Hydrogen storage materials: Traditional metallichydrogen storage materials provide a safe way to store hydrogen gas, but a low weightdensity (1.4 %) and operation complexity prohibit it from practical applications.Recently, carbon nano-tubes have attracted much research interest as a future hydrogenstorage material, but it still remains in the early investigation phase [3]. (c) Compressedhydrogen gas: It is expected to be the main stream for hydrogen storage in the near futureas it provides good volumetric and weight density (0.03 kg/L and 6%) and simplicity oftransportation and storage. Traditionally, compressed hydrogen gas is stored in metallic cylinders (Type Icylinder). The storage pressure for this type of cylinder is low (usually less than 25 MPa)and the capacity of hydrogen gas storage is limited. Also, hydrogen embrittlement canresult in micro-cracks and reduce the strength of the cylinder. The Type II cylinder isdeveloped by wrapping fiber-reinforced composite materials in the hoop direction on themetallic cylinder [4]. It reduces the weight of the cylinder significantly. However, thisstill does not meet the requirement of hydrogen storage capacity for automotives. Tofurther reduce the weight and increase the storage capacity, fully wrapped compositecylinders (Type III and Type IV) have been introduced. The cylinders are manufacturedby the filament winding technique. In this process, a liner is used as a mandrel and thehigh strength, low density composite (fiber strength 5-6 GPa, composite density 1.6g/cm3) is fully wrapped in both the helical and the hoop directions. The helical winding
13.
2produces helical layers to bear the axial loading, while the hoop winding generates hooplayers to carry circumferential loading. The liner serves as a gas barrier after the cylinderis manufactured. The Type III differentiates the Type IV by the material used for the liner(aluminum for Type III and polymer for Type IV). To obtain efficient storage capacity,the cylinders are designed for pressures as high as 5,000 to 10,000 psi and, hence, thefailure of the cylinder would lead to a catastrophic accident. In this context, safeinstallation and operation of high-pressure composite cylinders for hydrogen storage areof primary concern. To design the cylinder with the highest possible safety, reliabilityand minimum weight considerations, mechanics relevant to the behavior of the cylindermust be well understood. The early technique used for analyzing filament-wound composite cylinders is nettinganalysis [5-7]. This procedure has been widely used in the industry for its simplicity. Astatic equilibrium principle is applied to obtain the stress on the fiber by neglecting thecontribution of the resin matrix. Although this technique provides a concise way topredetermine some design parameters for cylinder prototypes, more detailed analysis isnecessary for examining and optimizing the high pressure composite cylinder forhydrogen storage under various operating conditions. Considering the effect of resin matrix, many studies have been focused on developingan analytical solution for composite cylinders under various loadings. Lekhnitskii [8] laidthe foundation for analyzing the anisotropic elasticity. Numerous authors [9-13]advanced the model for the stress analysis of cylinders under uniaxial, biaxial andcombined centrifugal pressure loadings in terms of stress functions. Later on, based on aplain-strain assumption, Akcay and Kaynak [14] analyzed closed-end cylinders underuniform thermal loading. Sayman [15] incorporated a general hydrothermal effect in themodel that is suitable for multi-layered thin/thick composite cylinders for the axiallysymmetric case under uniform or parabolic temperature distributions. Tabakov [16]developed a model to obtain exact solutions for the thick laminated anisotropic cylinderwith closed ends, but this model was limited to five layers and was not universal. In hislater work [17], a general model was developed by deriving the governing differentialequations instead of stress functions without considering the end effects and closing
14.
3plates. More recently, Chapelle and Perreux [18] extended the analytical method toanalyzing a Type III hydrogen cylinder by including plastic flow of the liner. The Finite Element Method (FEM) provides a convenient tool to analyze compositecylinders with consideration of nonlinearities, failure modes and various loadingconditions. A three dimensional finite element was developed by Hoa et al. [19] for thestrain analysis of fiber reinforced plastic vessels containing discontinuities such asmanhole connections or nozzles. Considering the change of winding angles through thethickness of helical laminates, finite element analyses were performed by Park et al. [20]through coding the winding angle to each solid element. Kabir [21] modeled the structureof the cylinder wall as an elastic, ideally plastic liner, reinforced with quasi-isotropicelastic composite. Tam et al. [22] analyzed the composite tank considering both materialand geometric nonlinearities. Gray and Moser [23] described a method which has beendeveloped to analyze filament-wound composite pressure vessels accounting for thehighly orthotropic nature of vessel structures. Kim et al. [24] employed a 3-D element tocompute stresses for optimizing the composite pressure vessel design. In addition,significant studies were conducted by several researchers [25-28] on the analysis ofcomposite pressure vessels with incorporating failure and progressive damage models inFE programs. The fracture and fatigue behavior of composite pipes and cylinders havealso been investigated by many authors [29-34] using both stress/strain criteria and directcrack-modeling techniques in finite element models.1.2. SCOPE AND OBJECTIVES Based on the literature survey, many researchers have used finite element method onthe study of composite vessels or pipes, but there is no significant research on theanalysis of Type III cylinders subjected to thermo-mechanical loading. In the case of fireimpingements, the previous studies have been carried out on flat composite panels andlack the capability of analyzing composite cylinders considering both mechanical andthermal damage. Furthermore, fracture failure is another essential factor for the safetyand design life-expectancy of the cylinder. Most of the previous studies have performedfracture analysis either on compressed natural gas cylinders or on pressure vessels usedfor aerospace. Intensive analysis has been conducted on metallic cylinders and a few are
15.
4related to cylinders with a metallic liner wrapped by composites. However, not muchresearch has been performed on composite hydrogen cylinders with consideration of theautofrettage effect. As an effort to develop the finite element model to predict the behavior of Type IIIhydrogen cylinders for the safety concern and design guidance, this study focuses onthree aspects. The first one is to develop a finite element model that can predict thefailure pressure of the cylinder subjected to combined thermal and mechanical loadings.The second one is to develop a comprehensive finite element model that can identifyfailure modes of the cylinder when it is attacked by fire impingement. The third one is toevaluate the performance of the cylinder containing liner cracks from the perspectiveview of fracture mechanics using finite element simulation technique. This dissertation has been prepared in the form of three parts corresponding to theaddressed problems. The first part is titled “Failure Pressure Prediction of Composite Cylinders forHydrogen Storage using Thermo-mechanical Analysis and Neural Network.” In thispart, a finite element simulation tool for the design of hydrogen storage cylinders hasbeen developed. The structural response of the cylinder is analyzed using laminated shelltheory accounting for transverse shear deformation and geometric nonlinearity. Acomposite failure model is used to evaluate the failure pressure. A back-propagationNeural Network model is developed based on the results of finite element analysis topredict the maximum failure pressure for arbitrary thermo-mechanical loading conditions. The second part is titled “Analysis of Composite Hydrogen Storage CylindersSubjected to Localized Flame Impingements.” In this part, a comprehensive non-linearfinite element model has been developed for predicting the behavior of compositehydrogen storage cylinders subjected to high pressure and localized flame impingements.The model is formulated in an axi-symmetric coordinate system and incorporates varioussub-models to capture the behavior of the composite cylinder under extreme thermo-mechanical loadings. Sub-models are implemented in ABAQUS commercial finiteelement code using user subroutines. Numerical results are presented for thermal damage,residual properties and profile of resin content of the cylinder wall.
16.
5 The third part is titled “Fracture Analysis of Hydrogen Storage CompositeCylinders with Liner Crack accounting for Autofrettage Effect.” In this part, aglobal-local finite element model is developed to investigate the axial surface flaws in theliner of high pressure composite cylinders for hydrogen storage using fracture mechanics.The effect of autofrettage process is studied due to its strong influence on the cylinderfracture behavior. The autofrettage process simulation is conducted in the global model.The local model, which is driven by the results of the global model, performs a detailedanalysis of the crack to assure accurate computation of fracture parameters. Results ofboth stress intensity factor (K) and J-integral are reported along the crack front in fourautofrettage levels and with different crack sizes. The plastic zone along the crack front isalso studied.1.3. CONCLUDING REMARKS In the first part, a doubly curved shell model accounting for transverse sheardeformation is used for the thermo-mechanical analysis of hydrogen composite storagecylinders. Temperature dependent material properties of the load carrying carbon/epoxylayer and geometry nonlinearity are also considered in the numerical model. Underuniform thermal loading, a temperature increase significantly raises the maximum failurepressure based on the Tsai-Wu failure criterion. Contrastively, the non-uniform thermalloading can cause an uneven load distribution and hence decrease the maximum failurepressure. The thickness ratio also plays an important role in determining the maximumfailure pressure and should be selected appropriately based on the thermal andmechanical loading conditions. A neural network model is developed and used to predictthe failure pressure. The performance of the trained neural network is then evaluated bycomparing the predicted values with those of testing cases. The results are in goodagreement. In the second part, a comprehensive finite element model has been developed toanalyze composite hydrogen storage cylinders subjected to high pressure and flameimpingements. The model considers the resin reaction, heat exchange between thehydrogen gas and liner, and the progressive failure process. A sub-laminate model hasbeen developed to reduce computational time. A temperature dependent material model
17.
6along with a failure model has been developed and implemented to accurately predictvarious failure modes for the hydrogen storage cylinder. Analysis of a typical highpressure composite hydrogen cylinder under fire exposure is conducted by using thedeveloped models. Parametric studies are done on heat exchange rate (between hydrogengas and the liner) and the size of the flame source. Stresses, temperature profile andfailure types are reported. The developed model can be used to accommodate varioustypes of thermal and mechanical loadings, lamina stacking sequence, and laminathickness to establish safe working conditions and design limits for hydrogen storagecylinders. In the third part, a global-local finite element model has been developed to predict thefracture behavior of high pressure composite cylinders for hydrogen storage. Simulationof the autofrettage process is carried out in the global model. Plastic hardening and theBauschinger effect are observed in the results. Both stress intensity factor (K) and J-integral are computed along the crack front in the local model with consideration ofautofrettage influence and crack size effect. It is found that the autofrettage processsignificantly improves the cylinder fracture performance and the smaller crack sizereduces the value of fracture parameters dramatically. The plastic zone around the cracktip is studied in terms of shape and size. The fracture behavior is discussed throughobservation of the plastic zone and the corresponding selection of parametriccharacterization is suggested. The current research can be extended in several ways for future work. The developedNeural Network model for failure pressure prediction can be applied to optimization ofcomposite lay-ups under arbitrary environmental temperature conditions. The second partof the model can be extended to multi-physics analysis by simulating the fluid field ofhydrogen gas in the cylinder. Pressure release device can be designed based on theprediction of simulation to minimize the hazard of cylinder failure when subjected toaccidental fire. The fracture model can be used as a tool for cylinder autofrettage processto obtain an optimum stress state to restrict crack growth in the liner. Also, the currentlydeveloped fracture model can be extended to predict the fatigue life of the cylinder andprovide guidance for material selection and lay-up optimization of the composite wall toachieve premium fracture performance.
18.
7 PAPER I: FAILURE PRESSURE PREDICTION OF COMPOSITE CYLINDERS FOR HYDROGEN STORAGE USING THERMO-MECHANICAL ANALYSIS AND NEURAL NETWORK ABSTRACT Safe installation and operation of high-pressure composite cylinders for hydrogenstorage are of primary concern. It is unavoidable for the cylinders to experiencetemperature variation, and significant thermal input (or flux) during the service. Themaximum failure pressure that the cylinder can sustain must be affected due to the natureof temperature dependent composites, integrity of the matrix and fibers and complexityof the cylinder design. Most of the analysis reported in high-pressure composite cylindersis based on simplified assumptions and does not account for complexities like thermo-mechanical behavior and temperature dependent material properties. In the present work,a comprehensive finite element simulation tool for the design of a hydrogen storagecylinder is developed. The structural response of the cylinder is analyzed using laminatedshell theory accounting for transverse shear deformation and geometric nonlinearity. Acomposite failure model is used to evaluate the failure pressure under various thermo-mechanical loadings. A back-propagation Neural Network (NNk) model is developed topredict the maximum failure pressure using the analysis results. The failure pressurespredicted from the NNk model are compared with those from testing cases. Thedeveloped NNk model is capable of predicting the failure pressure for any given loadingcondition.
19.
81. INTRODUCTION Composite high-pressure cylinders have potential application as hydrogen storagesystems in automotive, transportation, portable, and stationary storage systems due totheir light weight, simplicity of the storage and low cost for storage and transport ofhydrogen gas [1]. Typically, a composite high-pressure cylinder is made of a highmolecular weight polymer or aluminum liner that serves as a hydrogen gas permeationbarrier. A filament-wound, carbon/epoxy composite laminate over-wrapped outside ofthe liner provides the desired pressure load bearing capacity [2]. A vehicle fuel systemcylinder is capable of sustaining pressures of 5,000 psi or higher by taking advantage ofthe high strength and low specific weight of modern high performance composites. Inaddition, the maturation of the filament winding manufacturing process further reducesthe price to being practical and common for use in mass transportation systems. To design composite high-pressure cylinders with the highest possible safety,reliability and minimum weight considerations, the behavior of composite structuresunder various mechanical and thermal loadings, including localized and non-localizedflames, needs to be well understood. Studies have been conducted by various researchers[3-5] on the structure of hydrogen composite cylinders under mechanical loadings. Usingfinite element method as a powerful numerical tool, numerous studies have beenconducted on high-pressure cylinder analysis [6-8]. Compared to pure mechanicalloading, fewer studies have been conducted on hydrogen composite cylinders subjectedto thermal loads and combined thermo-mechanical loads [9, 10]. In the present study, a thermo-mechanical finite element model has been developedfor the analysis of hydrogen storage cylinders. The composite laminate wall of hydrogen
20.
9composite cylinder typically consists of helical and hoop laminated layers. Both theselayers, along with an aluminum liner, are considered for the analysis. During service,hydrogen composite cylinders unavoidably experience various thermal loadingscombined with high inner pressure. To account for working temperature variation in theservice, uniform temperature loadings ranging from 25C to 140 C are considered for theanalysis, above which the matrix begins to burn. During the gas filling process, the innertemperature can go up to around 100 C [10]. Hence, non-uniform thermal loadings havealso been included in the study. The variation of material properties with temperature issignificant for most composites. A temperature dependent material model has beendeveloped and implemented in commercial finite element code ABAQUS, using usersubroutines. A laminated shell theory [11, 12] accounting for out-of-plane shear strainsand geometric nonlinearity is used for the analysis. When considering the combination of various thermal loadings, winding angles andlay up configurations in the analysis, it is a tremendous task to optimize the cylinderdesign and predict maximum failure pressure through case-by-case simulation. A back-propagation Neural Network (NNk) model is then developed to predict the failurepressure using the results from a few typical finite element simulation cases. The trainingprocess consists of training the network with three sets of simulation results with variouswinding angles and thermal loadings. Once trained, the developed NNk model can beused for guidance and optimization of hydrogen cylinder design. Some testing cases,which are not included in the training sets, are utilized to compare with the predictedfailure pressure from the NNk model. A good agreement is found between failurepressures from testing cases and NNk model prediction.
21.
102. SHEAR DEFORMABLE SHELL THEORY A schematic of a hydrogen composite cylinder wall is shown in Figure 1. The innerliner is made of high molecular weight polymer or aluminum that serves as a hydrogengas permeation barrier. A filament-wound, carbon/epoxy composite laminate over-wrapped on the outside of the liner provides the desired pressure load bearing capacity[13]. In many current designs, a glass/epoxy layer is placed over the carbon/epoxylaminate to provide impact and damage resistance. The doubly curved shell theoryaccounting for out of plane shear deformations and geometric nonlinearity is used for theanalysis of composite hydrogen storage cylinders. A multilayered doubly curved shell is shown in Figure 2. The curved coordinatedsystem 1 , 2 , is used in space description. The coordinates 1 and 2 specify theposition on the middle surface, while measures the distance, along the outward normal,from the mid-surface to an arbitrary point on the shell. The displacement field can bewritten as: u( 1 , 2 , ) = (1 + ) u o ( 1 , 2 ) + 1 ( 1 , 2 ) (1.a) R1 v( 1 , 2 , ) = (1 + ) v o ( 1 , 2 ) + 2 ( 1 , 2 ) (1.b) R2 w ( 1 , 2 , ) = w o ( 1 , 2 ) (1.c)The non-linear strain-displacement relations based on Sanders’s shell theory can be givenas: o o εx= εx + ζ κ x ; εy = εy + ζ κ y o o o γ xy = γ xy + ζ κ xy ; γ yz = γ yz ; γ xz = γ xz (2)
22.
11where ε 0 and κ j are defined as: j 2 1 uo 1 w o 1 1 o ε = x + wo + 2 ; κx = α1 ξ1 R 1 2α1 ξ1 α1 ξ1 2 1 v 0 w 0 o 1 w o 1 2 ε y + 2 ; κy α 2 2 R 2 2α 2 ξ 2 α 2 2 1 vo 1 uo 1 w o w o 1 wo o γ xy = + + ; γo = yz + 2 - vo (3) α1 ξ1 α 2 ξ 2 2α1α 2 ξ1 ξ 2 α2 ξ 2 R2 1 w o o γ xz = + 1 - u o α1 ξ1 R1 1 2 1 1 1 vo 1 u o κ xy = + - co - α1 ξ1 α2 ξ 2 α1 ξ1 α 2 ξ 2 1 1 1 c0 = - ; dx = α1dξ1 ; dy = α 2 dξ 2 2 R1 R 2 In Eq. (3), u and v are the displacements in the direction of the tangents to the coordinatelines 1 and 2 , respectively, w is the displacement in the direction of the outwardnormal and 1 and 2 are the rotations. The stress-strain relation, accounting for thermal effects, in the shell coordinates for ak th layer can be expressed as [12]: x Q11 Q12 Q16 0 0 ε x xT Q Q Q26 0 0 ε y yT y 12 22 xy Q16 Q26 Q66 0 0 xy xyT (4) 0 0 0 Q44 Q45 yz yz xz k 0 0 0 Q45 Q55 k xz kwhere Qij are the transformed elastic coefficients, T is the given temperature distribution,and x , y , xy are the thermal expansion coefficients in the shell coordinates.
23.
12 The laminate constitutive equations can be obtained by integrating Eq. (4) over thethickness, and is written as: Nx A11 A12 A16 0 0 B11 B12 B16 ε0 NT x x N A 0 T y 12 A 22 A 26 0 0 B12 B22 B26 εy Ny N xy A16 A 26 A66 0 0 B16 B26 B66 γ0 NT xy xy 0 Q xz 0 0 0 A 44 A 45 0 0 0 γ xz 0 0 0 - (5) Q yz 0 0 A 45 A55 0 0 0 γ yz 0 Mx B11 B12 B16 0 0 D11 D12 D16 κx MT x B T My B22 B26 0 0 D12 D 22 D26 κy My 12 M xy κ MT B16 B26 B66 0 0 D16 D 26 D66 xy xy where N T and M T are thermal stress and moment resultants h/2 A ij Bij Dij h/2 Qij 1 z z 2 dz i, j 1, 2, 6 (6.a) h/2 Aij K i K j Qij dz i, j 4,5 (6.b) h/2 T T Nx , M x Q11 Q12 Q16 x T T h/2 N y , M y h / 2 Q12 Q22 Q26 y 1, z Tdz (6.c) N T , M T Q16 Q26 Q66 xy xy xy where K is a shear correction factor. Following the standard finite element procedure, the generalized displacements in anyelement are given by: u u v v N w w i (7) i 1 1 1 2 2 i where N is the number of nodes in the element and i are the interpolation functions.Substituting Eq. (7) in Eq. (3), the strains can be expressed as:
24.
13 B1 ; B2 ; B3 (8)The finite element equation is written as: K e e F e FTe (9)where , T T T K e B1T AB1 B1T BB2 B2 BB1 B2 DB2 B3 SB3 d ( Area ) T u v w e 1 2 F B e T 1 T N B2 M d ( Area) F B T e T 1 N T B2 M T d ( Area) TFor any given mechanical and temperature loadings, Eq. (9) can be assembled and solvedto determine displacements and stresses.3. COMPOSITE FAILURE MODEL The Tsai-Wu failure criterion is used for failure evaluation of hydrogen compositestorage cylinders [14]. Taking 1 as the fiber direction and 2 and 3 as transversedirections, the Tsai-Wu failure criterion can be expressed as: 2 2 2 I F F1 11 F2 22 F11 11 F22 22 F44 23 2 2 (10) F55 13 F66 12 2 F12 11 22 1.0The coefficients in Eq. (10) are defined as: 1 1 1 1 1 F1 , F2 , F11 , Xt Xc Yt Yc Xt Xc 1 1 1 1 F22 , F44 2 , F55 2 , F66 2 , YtYc S 23 S13 S12
25.
14 1 1 1 1 1 1 1 2 F12 2 1 biax biax 2 biax X t X c Yt Yc X t X c YtYc or F12 f F11F22 ( 1 f 1 )where, X t and X c are tensile and compressive stress strengths along the fiber direction,Yt and Yc are tensile and compressive stress strengths in the transverse fiber direction,S 23 , S13 and S12 are the maximum shear strengths in corresponding planes, biax is theequi-biaxial stress at failure and f is an experience coefficient.4. MATERIAL PROPERTIES Mechanical and thermal properties of fiber reinforced composites vary significantlywith temperature. As the carbon/epoxy laminate carries the pressure loading from thehydrogen gas, the effect of temperature on its material properties cannot be ignored. Themoduli and thermal expansion coefficients are dependent on temperature. For HFGCU125 carbon/epoxy, the temperature dependent material properties are given by [15]: E1= 0.066 T + 128 (GPa) (25C < T < 140C) E2 = 0.064 T + 10.67 (GPa) (25C < T < 140C) G12 = 0.034 T + 5.39 (GPa) (25C < T < 140C) (11) 12 = 0.0005 T + 0.44 (25C < T < 140C) α1= (0.0003 T2 0.04 T + 2.09) × 10-6 (25C < T < 140C) α2 = (0.0041 T2 0.23 T + 32.2) ×10-6 (25C < T < 140C)
26.
15 Furthermore, G13 is taken as G12, and G23 is assumed as 0.7G12. The ultimatestrengths of carbon/epoxy do not change much with this temperature range and areassumed to be constant and are listed in Table 1. The material properties for glass/epoxyare listed in Table 2. The outer most glass/epoxy layer is primarily used for protection ofthe load bearing carbon/epoxy lamina. Hence temperature dependent material propertiesare not used for the glass/epoxy layers. Properties of the innermost aluminum liner arelisted in Table 3.5. FINITE ELEMENT SIMULATION ABAQUS is an integrated and open-ended Finite Element Analysis code, which iswidely used by the industry as well as researchers for the flexibility of implementing userdefined subroutines and its powerful nonlinear solver. With those features, the userdefined problem can be built up by combination of the basic frames provided by theABAQUS code and user model specialties implementing subroutines. All the modelingfeatures described in this work have been thus implemented in this code. A laminatedshell element, based on doubly curved shell theory, accounting for membrane, bendingand membrane-bending coupling and transverse shear effects, is suitable for modelingboth thin and thick laminated composites. For this purpose, the laminated composite wallof the cylinder is modeled by using a doubly curved 8-node shell element (S8R). In orderto estimate the failure pressure of the cylinder, it is necessary to include a failurecriterion. Tsai-Wu failure theory is utilized to check and report the ply-by-ply laminatefailure by using a user subroutine UVARM. In addition, the temperature dependentmaterial properties are incorporated in the model by using subroutine USDFLD so that, at
27.
16each integration point, the material properties are determined by the given temperature.The orientation of each element at every ply is handled by subroutine ORIENT accordingto the winding pattern. The cylinder is modeled and meshed using the ABAQUS/CAEpreprocessor as shown in Figure 3. Due to the symmetry, 1/8th of the cylinder isconsidered for the analysis. The comprehensive model is then solved by using theABAQUS/standard solver with geometric nonlinearity considered. The dimensions considered in the present cylinder analysis are based on a typicaldesign from the literature [13]. The outer radius of the cylinder is taken as Rout = 0.25 mand the inner radius Rin = 0.22 m (Figure 1). The pressure bearing carbon/epoxy laminateconsists of 24 plies resulting in a composite shell of thickness 28 mm. The protectiveglass/epoxy layer and liner are 2 mm and 2.5 mm thick respectively. The cylinder issubjected to an internal pressure that gradually increases until failure occurs in the firstply. To manufacture closed cylinders, two types of winding patterns are usually used:hoop and helical/polar windings. The thickness ratio R (total thickness of helicallaminate/total thickness of hoop laminate) affects the failure pressure of the cylinder anda range of 0.1 to 2.0 is studied. The winding angle of laminae also affects the failurepressure of the cylinder and a range of 10◦ to 30◦ for helical winding and 89o for hoopwinding has been considered based on manufacturing feasibility. The plies in theprotection laminate are oriented as 45 angle ply.
28.
176. NEURAL NETWORK MODEL A feedforward back-propagation Neural Network (NNk) is used to predict the failurepressure of a hydrogen cylinder. A schematic of the NNk is shown in Figure 4. Therelationship of failure pressure and the inputs (thickness ratio R , temperature inside thecylinder Tin , temperature outside the cylinder Tout , and winding angle ) is modeled by atwo-layer (hidden layer and output layer) network. Each layer consists of a number ofprocessing units, with an activation function, known as neurons. For faster training and Trobust NNk, inputs are scaled to a desirable range by a designed transfer function finbefore entering the input layer. Inputs are passed through weighted connections to thehidden layer and then to the output layer. The output P is, finally, scaled back to failure Tpressure P by a designed transfer function f out . The number of neurons in the hiddenlayer and the characterizing weights and biases in the model are determined by trainingthe NNk. The input transfer function T fin ( I i ) I i ai bi (12)whereI i are input variables ( i 1, 2,3and 4 corresponding to R, Tin , Tout and respectively) n nai max min Iimax I imin bi nmin Min{ai I i }[ nmin nmax ] is the desired scale range and is taken as [-1 1] and I i are input training pattern vectors.
29.
18 Normalized input variables I i are given by T I i fin ( Ii ) (13) The activation function in the hidden layer is the Log-sigmoid function 1 f h ( x) (14) 1 e x The activation function in the output layer is the Pureline function f o ( x) x (15) The normalized failure pressure P is given by [16] N 4 h P W1oj f h W ji Ii b h bo j (16) j 1 i 1 where N is number of neurons in the hidden layer W1oj are weights in the output layer h W ji are weights in the hidden layer bo is bias in the output layer and b h are biases in the hidden layer j The output transfer function T f out ( I i ) P b / a (17)where n n a max min P max P min , i 1, 2,3, and 4 b nmin Min{au P} , i 1, 2,3, and 4
30.
19 and P is the output training pattern vector. The final failure pressure P is given by T P fout ( P) (18) Training consists of providing a set of known input-output pairs (or patterns) to thenetwork. Back-propagation learning process has two passes through the network: aforward calculation pass and an error back-propagation pass. In the forward pass, inputpatterns broadcast from input layer to output layer in order to generate the actual resultsof network. During the backward propagation, weights in each node are iterativelyadjusted based on the errors using the gradient descent equations. The procedure isrepeated until convergence is achieved. In this study, the input-output sets are obtainedfrom simulation results. The model is trained in MATLAB NNk tool box. The fasttraining Levenberg-Marquardt Algorithm is adopted in the training process.7. RESULTS AND DISCUSSION Five configurations of helical and hoop laminas shown in Table 4 are investigated inthis study. Case studies are conducted on composite cylinders with various thermalloadings and lay-up patterns. Failure pressures as a function of thickness ratio R underuniform thermal loadings for Cases 1-3 are shown in Figures 5(a-c) respectively. The rateof increase in failure pressure is higher at higher temperatures. This reflects thenonlinearity of thermal expansion coefficients with variation in temperature. For all thethree cases considered, the failure pressure increases with increase in temperature. Incomparison with Cases 2 and 3, the peak failure pressure is slightly higher than that ofCase 1. Similar results are shown in Figures 6(a-c) with gradient thermal loading. In
31.
20comparison with the uniform thermal loadings, the peak failure pressure is not evident forsome of the inner temperatures considered in figure 5(b). In those cases, all hoop laminaeare placed over helical laminae with inner temperature higher than outer temperature.Then thermal strain, arising from thermal expansion, becomes larger in all helicallaminae which cause hoop laminae to carry most of the axial loadings. Without helicallaminae sustaining major part of the axial loading, the peak pressure then disappears atlower thickness ratio area. With increasing thickness ratio, the axial-load bearing capacityof the hoop laminae increases thus resulting in the rise in failure pressure. Thisphenomenon cannot be observed in Figures 6(b-c) because the helical and hoop laminaeare laid alternatively. From Figures 6(a-c), with inner temperature increasing (from 25oCto 140oC), the failure pressure rises till it reaches the set temperature (50oC) of outsidewall, and then starts to decrease. Also it can be observed that the failure pressuredecreases as the gradient of the non-uniform temperature increases. By comparison of Cases 1, 2 and 3, the alternative lay up pattern (in Cases 2 and 3)can result in higher failure pressure than that of non-alternative lay up (in Case 1), whencylinder is experiencing uniform thermal loading and no significant increase is observedin gradient thermal loading. However, in Case 1, the location of peak pressure varies a lotin comparison with that of Cases 2 and 3 under gradient thermal loading. This largevariation might bring down the failure pressure at optimum thickness ratio whenconsidering various thermal loadings in design. There is no significant difference that canbe observed between Case 2 (constant winding angle in helical laminate) and Case 3(gradually increased winding angle in helical laminate). To study the effect of helicalwinding angle pattern on failure pressure, Cases 2, 4 and 5 ( [±20o /±89o ]6 ,
32.
21[±10o /±89o ]6 and [±30o /±89o ]6 ) are compared with different thickness ratios (R) asshown in Figure 7. For the same thickness ratio, higher peak failure pressure is observedfor smaller winding angle. Figure 8 shows the Tsai-Wu failure indicator for each helical and hoop ply in Case 2for thickness ratio, R=0.5. Curves 1 and 2 (T25-25 and T140-140 respectively) illustratethe ply failure under uniform thermal loadings while curves 3 and 4 (T25-100 and T100-25 respectively) show the failure under gradient thermal loadings (T25-25 impliesTin=25oC and Tout = 25oC). With uniform thermal loading at 140oC, the curve is observedto be flat, which implies that all the helical and hoop laminae fail simultaneously.However, at uniform thermal loading of 25oC, the helical laminae tend to fail first. Whensubjected to non-uniform thermal loading, a large slope is observed in the curves. Theinner layers fail first for T25-100 ( Tin = 25oC and Tout =100oC), while the outer layers failfor T100-25 ( Tin = 100oC and Tout =25oC). This asynchronous behavior of inner or outerlayers during failure must cause a significant drop in maximum failure pressure,assuming that the cylinder fails when any one of the laminae fails. The network is trained by using the simulation results from Cases 2, 4 and 5 shown inTable 4. There are 12 neurons used in the neural network (NNk) model and the trainingratio is set to 0.01. After the network gets converged, the model parameters are obtainedand are listed in Tables 5 and 6. The network model is then capable of predicting thefailure pressure by providing the network inputs ( R , Tin , Tout and ). To evaluate theperformance of NNk prediction, six testing cases (shown in Table 7) are studied. Thetesting data from ABAQUS simulation results, for winding angles not used before (15oand 25o), are used to compare the predicted results from the trained neural network. The
33.
22performance of the NNk is then illustrated in Figures 9(a-b), and the maximum errors arereported for each case in Table 7. It can be seen that the simulation results are in goodagreement with the results predicted by the NNk model. The trained network can,therefore, be used to predict any failure pressure within the trained ranges of temperature,winding angle and thickness ratio.8. CONCLUSIONS A doubly curved shell model accounting for transverse shear deformation is used forthermo-mechanical analysis of hydrogen composite storage cylinders. Temperaturedependent material properties of the load carrying carbon/epoxy layer and geometricnonlinearity are also considered in the numerical model. Five typical cases have beenconsidered and the analysis is carried out by applying uniform/non-uniform thermalloading and internal pressure loading. The Tsai-Wu failure criterion is employed topredict the failure pressure by checking the failure, layer by layer. Under uniform thermalloading, a temperature increase significantly increases the maximum failure pressure.Contrastively, the non-uniform thermal loading can cause an uneven load distribution andhence decrease the maximum failure pressure. The thickness ratio also plays an importantrole in determining the maximum failure pressure and should be selected appropriatelybased on the thermal and mechanical loading conditions. A neural network (NNk) modelis developed and used to predict the failure pressures. The performance of the trainedneural network is then evaluated by comparing the predicted values with those of testingcases and the results are in good agreement.
34.
23 REFERENCES[1] N. Takeichia, H. Senoha, T. Yokotab, H. Tsurutab, K. Hamadab, H. Takeshitac, H. Tanakaa, T. Kiyobayashia, T. Takanod and N. Kuriyamaa, “Hybrid Hydrogen Storage Vessel, A Novel High-pressure Hydrogen Storage Vessel Combined with Hydrogen Storage Material,” International Journal of Hydrogen Energy, Vol. 28, pp. 1121-1129, 2003.[2] C. Liang, H. Chen and C. Wang, “Optimum Design of Dome Contour for Filament- wound Composite Pressure Vessels Based on a Shape Factor,” Composite Structures, Vol. 58, pp. 469-482, 2002.[3] V. V. Vasiliev, A. A. Krikanov and A. F. Razin, “New Generation of Filament- wound Composite Pressure Vessels for Commercial Applications,” Composite Structures, Vol. 62, pp. 449-459, 2003.[4] P. Y. Tabakov and E. B. Summers, “Lay-up Optimization of Multilayered Anisotropic Cylinders Based on a 3-D Elasticity Solution,” Computers and Structures, Vol. 84, pp. 374-384, 2006.[5] J. Park, C. Hong, C. Kim and C. Kim, “Analysis of Filament Wound Composite Structures Considering the Change of Winding Angles Through the Thickness Direction,” Composite Structures, Vol. 55, pp. 63-71, 2002.[6] M. Z. Kabir, “Finite Element Analysis of Composite Pressure Vessels with a Load Sharing Metallic Liner,” Composite Structures, Vol. 49, pp. 247-255, 2000.[7] D. L. Gray and D. J. Moser “Finite Element Analysis of a Composite Overwrapped Pressure Vessel,” 40th AIAA/ASME/SAE/ASEE Joint Propulsion Conference and Exhibit, Fort Lauderdale, FL, AIAA 2004-3506, pp.1-15, July 11-14, 2004.[8] I. H. Akcay and I. Kaynak, “Analysis of Multilayered Composite Cylinders under Thermal Loading,” Journal of Reinforced Plastics and Composites, Vol. 24, pp.1169-1179, 2005.[9] O. Sayman, “Analysis of Multi-layered Composite Cylinders under Hygrothermal Loading,” Composites: Part A, Vol. 36, pp. 923-933, 2005.[10] J. M. Schneider, “Gaseous Hydrogen Station Test Apparatus: Verification of Hydrogen Dispenser Performance Utilizing Vehicle Representative Test Cylinders,” SAE World Congress & Exhibition, Detroit, MI, pp.1-10, April 2005.
35.
24[11] K. Chandrashekhara and A. Bhimaraddi, “Thermal Stress Analysis of Laminated Doubly Curved Shells using a Shear Flexible Finite Element,” Computers and Structures, Vol. 52, pp. 1023-1030, 1994.[12] K. Chandrashekhara and T. Schroeder, “Nonlinear Impact Analysis of Laminated Cylindrical and Doubly Curved Shells,” Journal of Composite Materials, Vol. 29, pp. 2160-2179, 1995.[13] F. Mitlitsky, A. H. Weisberg and B. Myers, “Vehicular Hydrogen Storage Using Lightweight Tanks,” Proceedings of the U.S. DOE Hydrogen Program Review NREL/CP-570-28890, 2000.[14] S. W. Tsai and E. M. Wu, “A General Theory of Strength for Anisotropic Materials,” Journal of Composite Materials, Vol. 5, pp. 58-80, 1971.[15] K. J. Yoon and J. Kim, “Prediction of Thermal Expansion Properties of Carbon/Epoxy Laminae for Temperature Variation,” Journal of Composite Materials, Vol.34, pp. 90-100, 2000.[16] M. T. Valoor and K. Chandrashekhara, “A Thick Composite Beam Mode for Delamination Prediction by the Use of Neural Networks,” Composite Science and Technology, Vol.60, pp. 1773-1779, 2000.
36.
25 LIST OF TABLESTable 1 Ultimate strength of carbon/epoxy compositeTable 2 Mechanical and thermal properties of S-glass/epoxyTable 3 Mechanical and thermal properties of Aluminum Alloy 6061-T6Table 4 Lay-up configurations for various winding patternsTable 5 Weights and biases for trained neural networkTable 6 Scale constants for trained neural networkTable 7 Testing cases and maximum error of prediction
37.
26 LIST OF FIGURESFigure 1 Structure scheme of hydrogen storage cylinderFigure 2 Doubly curved shell and coordinate systemFigure 3 Finite element model of hydrogen cylinderFigure 4 Feedforward back-propagation Neural Network architectureFigure 5(a) Uniform thermal loading with Tin=Tout (in Case 1)Figure 5(b) Uniform thermal loading Tin=Tout (in Case 2)Figure 5(c) Uniform thermal loading Tin=Tout (in Case 3)Figure 6(a) Gradient thermal loading with Tout=50oC (in Case 1)Figure 6(b) Gradient thermal loading with Tout=50oC (in Case 2)Figure 6(c) Gradient thermal loading with Tout=50oC (in Case 3)Figure 7 Failure pressure with inside temperature variation (Tout=25oC)Figure 8 Ply-by-ply failure predictions under various thermal loadingsFigure 9(a) Comparison of failure pressures from NNk and ABAQUS at = 15oFigure 9(b) Comparison of failure pressures from NNk and ABAQUS at = 25o
43.
32Table 6 Scale constants for trained neural network i ai bi a b 1 1.05263 -1.10526 0.05090 -1.96068 2 0.01739 -1.43478 3 0.01739 -1.43478 4 0.10000 -2.00000
44.
33Table 7 Testing cases and maximum error of prediction Testing Inputs Max. Error case Tin (oC) Tout (oC) θ (Degree) (%) 1 40 40 15 1.32 2 30 80 15 -1.54 3 130 40 15 1.23 4 40 40 25 1.11 5 30 80 25 -2.40 6 130 40 25 -1.00
45.
34 Tout Glass/Epoxy 26:-450 Glass/Epoxy 25: 450 R out Carbon/Epoxy 24: 89 0 Carbon/Epoxy 23:-890 Carbon/Epoxy 2:-100 Carbon/Epoxy 1: 100 Aluminum Tin R in PressureFigure 1 Structure scheme of hydrogen storage cylinder
46.
35Figure 2 Doubly curved shell and coordinate system
47.
36Figure 3 Finite element model of hydrogen cylinder
48.
37 b1h fh h W 11 R b2h o W11 R Tin fh bo Tin T fin o fo P f T Tout W12 out P Tout h W1o N h b N WN 4 fh Input layer Hidden layer Output layerFigure 4 Feedforward back-propagation Neural Network architecture
49.
38Figure 5(a) Uniform thermal loading with Tin=Tout (in Case 1)
50.
39Figure 5(b) Uniform thermal loading Tin=Tout (in Case 2)
51.
40Figure 5(c) Uniform thermal loading Tin=Tout (in Case 3)
52.
41Figure 6(a) Gradient thermal loading with Tout=50oC (in Case 1)
53.
42Figure 6(b) Gradient thermal loading with Tout=50oC (in Case 2)
54.
43Figure 6(c) Gradient thermal loading with Tout=50oC (in Case 3)
55.
44Figure 7 Failure pressure with inside temperature variation (Tout=25oC)
57.
46Figure 9(a) Comparison of failure pressures from NNk and ABAQUS at = 15o
58.
47Figure 9(b) Comparison of failure pressures from NNk and ABAQUS at = 25o
59.
48 PAPER II: ANALYSIS OF COMPOSITE HYDROGEN STORAGE CYLINDERS SUBJECTED TO LOCALIZED FLAME IMPINGEMENTS ABSTRACT A comprehensive non-linear finite element model is developed for predicting thebehavior of composite hydrogen storage cylinders subjected to high pressure andlocalized flame impingements. The model is formulated in an axi-symmetric coordinatesystem and incorporates various sub-models to describe the behavior of the compositecylinder under extreme thermo-mechanical loadings. A heat transfer sub-model isemployed to predict the temperature evolution of the composite cylinder wall andaccounts for heat transport due to decomposition and mass loss. A compositedecomposition sub-model described by Arrhenius’s law is implemented to predict theresidual resin content of the thermal damaged area. A sub-model for material degradationis implemented to account for the loss of mechanical properties. A progressive failuremodel is adopted to detect various types of mechanical failure. These sub-models areimplemented in ABAQUS commercial finite element code using user subroutines.Numerical results are presented for thermal damage, residual properties and the profile ofthe resin content in the cylinder. The developed model provides a useful tool for safedesign and structural assessment of high pressure composite hydrogen storage cylinders.
60.
491. INTRODUCTION High pressure composite cylinders for hydrogen storage are typically made with ahigh molecular weight polymer or aluminum liner that serves as a hydrogen gaspermeation barrier. A filament-wound, carbon/epoxy composite laminate over-wrappedon the outside of the liner provides the desired pressure load bearing capacity. Due to theflammable nature of polymer-reinforced composites, there is a high risk of failure of thecomposite hydrogen storage cylinder under accidental fire exposure. As the stiffness andstrength of composites are temperature dependent, the high pressure (usually 34.5 MPa to70.0 MPa) in the cylinder can result in catastrophic failure. Therefore, assessment ofstructural integrity of high pressure composite hydrogen storage cylinders subjected tofire exposure is necessary for safe cylinder design. Many investigations have been conducted by various researchers [1-4] on thebehavior of high pressure composite cylinders under mechanical loadings. Using finiteelement methods, numerous studies have been performed on high-pressure vesselanalysis [5-7]. Compared to pure mechanical loading and pure thermal loading, therehave been few studies on the composite cylinders subjected to the combined thermal andmechanical loads [8-9]. However, those models only consider the temperature rangebefore composite decomposition occurs and fall short of providing capability to assessthe behavior of cylinders subjected to fire impingement. To study fire effect oncomposites, different one-dimensional thermal models have been developed to predict thetemperature and the residual resin content as a function of time [10-12]. These modelsaccount for heat transfer by conduction, resin decomposition, and the cooling effect ofvolatile products passing through the laminate. Therefore, to characterize the fire
61.
50response of high pressure hydrogen composite cylinders, mechanisms of mechanicaleffect, thermal effect and decomposition have to be considered. In this paper, a coupled thermo-mechanical finite element model has been developedto simulate composite hydrogen storage cylinders subjected to high pressure and heat fluxon the wall surface. The model is formulated in an axi-symmetric coordinate systemwhich accounts for out-of-plane stresses and reduces computational cost dramatically.When the polymer materials are exposed to a sufficiently high temperature (200-300°C),decomposition reactions and thermo-chemical expansion begin to occur and the resinsystem degrades to form gaseous products and carbonaceous char. In order to incorporatethis phenomenon, the thermal model is built to account for gas convection and heatgeneration due to decomposition in addition to conduction of the composite, convectionand radiation of surface. The fire source is modeled as a constant heat flux throughout thesimulation. The inner pressure of the cylinder is dependent on the temperature ofhydrogen gas which is modeled as a sink temperature. The variation of materialproperties with temperature is significant for composites, especially at high temperatures.A temperature dependent material model has been developed and implemented. Hashin’stheory is used as a progressive failure criterion to predict different types of failure (matrixcracking and fiber breakage). These models are developed and implemented in acommercial finite element code ABAQUS, using user subroutines. A typical highpressure hydrogen composite cylinder is simulated using the developed model and resultsfrom the parametric study are reported.
62.
512. MODELING OF HIGH PRESSURE COMPOSITE HYDROGEN STORAGECYLINDERS A strong sequentially coupled thermal-stress analysis approach is implemented forpredicting the behavior of composite hydrogen cylinders subjected to flameimpingements and high internal pressure. At each increment, the temperature profile isobtained using the thermal and resin reaction models. The temperature field is thenimported to the mechanical model with material damage information from the previousincrement. The pressure of the inner cylinder is updated based on the heat absorption ofhydrogen gas, which is computed from the temperature profile. The thermal andmechanical models are solved sequentially in each increment. As the wall consists of alarge number of laminae, modeling each lamina will cause extraordinary computationalcost, especially when thermal and damage models are also incorporated. Hence, ahomogenization technique is used to smear several laminae to a sub-laminate as in Figure1. The equivalent moduli of the sub-laminate are used in the formulation of the finiteelement model.2.1 Thermal Model The high temperature will cause resin decomposition of the cylinder composite wall.The decomposition rate of the resin is usually represented by Arrhenius’s law and can beexpressed as [13]: A exp( EA / RT ) (1) twhere, – density
63.
52 t – time T – temperature A – pre-exponential factor E A – activation energy R – gas constant Material constants A and EA are determined using Differential Scanning Calorimetry.In consideration of the resin reaction, the heat transfer equilibrium equation has toinclude resin decomposition energy and vaporous migration energy. Since the dimensionin the thickness direction is much less than that of hoop and axial directions, the vaporousgas is only assumed to transfer in thickness direction. The axi-symmetric heat diffusionequation can be written as [14]: T T 1 T T T C p kr kr kz mg C pg t r r r r z z r t Q hcom hg (2)where, C p – specific heat of the composite k – thermal conductivity r – displacement through the thickness mg – gas mass flux C pg – specific heat of the gas Q – heat of decomposition hcom – enthalpy of the composite hg – enthalpy of hydrogen gas
64.
53 The mass flow direction of the gas generated in the laminate is towards the hot face ofthe laminate. The total mass flux of the generated gas at a specific spatial location in thelaminate is the sum of the gas mass flux generated from the inner face to this spatiallocation. The gas mass flux at any spatial location can be calculated as: rh mg drh (3) tW t where, rh – distance from the hot face tW – wall thickness of the composite2.2 Sub-laminate Model The principle of sub-laminate (Figure 1) homogenization is based on the assumptionthat the in-plane strains and the interlaminar stresses through the thickness are constant[15-18]. The lamina stress-strain relationship in a global coordinate can be written as: o Coo Coi o (4) i Coi Cii i where, Coo , Coi and Cii are sub matrices of global stiffness matrix, Coi is the transpose ofCoi , o and i are out-of-plane and in-plane stresses respectively, o and i are out-of-plane and in-plane strains respectively. represents the term is constant through thelaminate. Partially inverting Eq. (4) yields: o Coo1 Coo1Coi o (5) 1 i Coi Coo 1 Coi Coo Coi Cii i After averaging, Eq. (5) can be expressed as:
Be the first to comment